International Journal of Engineering Research Volume No.2, Issue No.2, pp : 161-166
(ISSN : 2319-6890) 01 April 2013
Kinetic and Electrical Conductivity Measurement Study of SDBF Resin Dhanraj.T.Masram1, K.P.Kariya2, N.S.Bhave3 1
Department of Chemistry, University of Delhi, Delhi-110007, India. Department of Chemistry, VMV commerce JMT Arts & JJP Science College, Nagpur-440008. 3 Department of Chemistry, Rashtrasant Tukadoji Maharaj Nagpur University, Nagpur-440033. firstname.lastname@example.org, Mob: +919958552279. Abstract: 2
Resin SDBF has been synthesized by the condensation of salicylicacid and diaminobenzoicacid with formaldehyde and hydrochloricacid as catalyst. Thermal degradation curve has been discussed which shows four decomposition steps. Detailed thermal degradation studies of the resin have been carried out to ascertain its thermal stability. Sharp– Wentworth and Freeman–Carroll methods have been used to calculate activation energies and thermal stability. The activation energy (Ea) calculated by using the Sharp– Wentworth (17.2 kJ/mol) has been found to be in good agreement with that calculated by Freeman–Carroll (26.80 kJ/mol) method. Thermodynamic parameters such as free energy change (ΔF), entropy change (ΔS), apparent entropy change (S*) and frequency factor (Z) have also been evaluated on the basis of the data of Freeman–Carroll method. The order of reaction (n) is found out to be 1.03. Electrical conductivity measurements have been also conceded to ascertain the semiconducting nature of the resin.
Keywords: Resin; synthesis, Thermal properties, Activation energy, Electrical conductivity.
1. INTRODUCTION The resins offer novelty and versatility; hence they occupy the pivotal position in the field of material science. The progress in the field resins has been extremely rapid, as they generally useful in packaging, adhesives and coatings in electrical sensors and organometallic semiconductors [1-4]. Phenolic resins have a large number of practical applications in electronic controls, insulating materials, protective adhesives, aerospace industries etc. because of their high thermal stability, heat and chemical resistance and electrical insulation properties [5-7].Various researchers have been studied the applications of resins of substituted phenols and formaldehyde [8-10]. 2-Hydroxyaceto phenone and its substituted derivatives have been condensed with formaldehyde to produce heat and light stabilizers. Resins of salicylic acid,
thiourea with trioxane and p-hydroxybenzoic acid, thiourea with trioxane have been reported in the literature [11-15]. Semiconductors are the most important ingredients of modern electronics. The concerted research effort was carried out to aim at developing an organic material that would posses the good electrical properties as the inorganic semiconductors. In the early days the prime attention was placed on the synthesis of highly conductive polymers, preferably of high molecular weight and the measurement of their electronic conductivity properties i.e. conductivity, mobility, thermoelectronic power, etc. The resins are well known for their behavior as semiconductors though carrier mobility in them usually is very low [16-18]. Kand a et al reported the rubeanato –copper semiconductive polymers and studied their AC and DC conductivity . Dhawan and coworkers reported the conducting polymers predicted to be the futuristic materials for the development of light emitting diodes, antistatic and EMI materials, sensors, opto- electronic devices and rechargeable batteries due to their unique conduction mechanism and greater environmental stability . In our laboratory, study on the synthesis of materials for high thermal stability and electrical conductivity measurements of resins derived from salicylicacid / p-hydroxybenzoicacid, diamide / urea / thiourea with formaldehyde [6, 7, 12-14, 2124]. The present communication deals with thermal degradation and electrical conductivity properties of a newly synthesized resin derived from salicylicacid, diaminobenzoicacid and formaldehyde. Methods for the estimation of kinetic parameters from thermo gravimetric studies are generally based on the assumption that the Arrhenius equation is valid with thermal and diffusion barriers are negligible. After treating the thermal degradation data with Sharp–Wentworth (SW) and Freeman– Carroll (FC) methods, activation energy and kinetic parameters such as ΔF, ΔS, Z, S* and n (order of reaction) have been evaluated . For the electrical conductivity measurement study the DC resistivity of the SDBF resin have been measured by applying a constant voltage (50 volts) across the pellets. The
International Journal of Engineering Research Volume No.2, Issue No.2, pp : 161-166 temperature dependence of the electrical conductivity of the resin has been plotted. The energy of activation (Ea) of electrical conduction is calculated from the slope of the plots. Electrical conductivity of the resin has been studied with increase in temperature.
(ISSN : 2319-6890) 01 April 2013 NH2
1200C Diaminobenzoic acid
+ 2n H2O
2. EXPERIMENTAL CH2
2.1 Chemicals All Chemicals were AR grade. Salicylicacid, diaminobenzoicacid and formaldehyde were purchased from Aldrich Chemical Co., USA. DMF and DMSO were used as solvent of HPLC grade. 2.2 Instruments Used Thermogravimetric analyses (TGA) of resin sample has been carried out by using Perkins Elmer TGS-ll thermal analyzer at heating rate of 100C per minute and in air atmosphere upto 8000C. The thermogram was recorded at Sophisticated Instrumentation Centre for Applied Research and Testing (SICART), Vallabh Vidyanagar, Gujrat. The electrical resistivity of the resin was measured with help of Hewlett-Packard 4192 Impendance Analyser 5Hz-13MHz at Department of Physics, Rashtrasant Tukadoji Maharaj Nagpur University, Nagpur over a wide range of temperature i.e. from 313-423 K. 2.3 Synthesis and Characterization of SDBF Resin A mixture of salicylicacid, diaminobenzoicacid and formaldehyde was taken in the ratio of 1: 1: 2 with 2 mol–L-1 hydrochloricacid as catalyst in a round bottom flask. The flask was fitted with water condenser and heated in an oil bath at 1200C for 7 hours with occasional shaking. The resinous solid product obtained was immediately removed from the flask as soon as the reaction period was over and then purified. The resinous product so obtained was repeatedly washed with cold distilled water dried in air and powdered with the help of agated mortar and pestle. The powder was washed many times with hot water to remove unreacted monomers. The air-dried powder was extracted with diethyl ether and followed by washing with the petroleum ether to remove salicylicacid diaminobenzoicacid copolymer, which might be present along with SDBF resin.
Scheme: Synthesis of SDBF Resin 3. THERMOGRAVIMETRY Thermal analysis method is associated with a change in weight with respect to temperature. Heating is performed under strictly controlled conditions and can reveal changes in structure and other important properties of the material being studied. In non-isothermal or dynamic TGA the sample is subjected to conditions increase in temperature at linear rate [28, 29]. Freeman–Carroll and Sharp- Wentworth methods have been employed for the calculation of kinetic parameters of the newly synthesized resin with help of dynamic TG curve [6,12,14,22-24,27]. The advantage of Freeman and Carroll method that in one single stage by keeping heating rate constant both the order of reaction and energy of activation can calculated in a single experiment. The following expression is used to evaluate various kinetic parameters: log dw / dt Ea (1 / T ) n . log Wr 2.303 R log Wr
Hence, a plot of
dw log dt vs. (1/ T ) log Wr log Wr
should give a
straight line with an intercept on y-axis equal to the value of n (the order of reaction) and the slope m = E / 2.303R. Where, dw/dt is the rate of change of weight with time and in expression Wr = Wc –w, Wc is the weight loss at the completion of the reaction, w is the total weight loss upto the time t and T is the temperature in k. The following expression is used to evaluate Ea with SharpWentworth method: log
Ea ( dc / dT ) 1 log( A / ) (1 c ) 2.303 R T
Where, dc/dt is the rate of change of mass with time t, T is the temperature and = T/dt.
International Journal of Engineering Research Volume No.2, Issue No.2, pp : 161-166
Fig.1: Thermogram of SDBF resin 4. ELECTRICAL CONDUCTIVITY The resins are well known for their behavior as semiconductors though carrier mobility in them usually is very low. This is due to the difficulty which electrons experience in jumping from one molecule to another and so the carrier mobility in compounds of these kind increases with increase in molecular size [16-20].The measurements involved following steps. 4.1 Preparation of pellets for Resistance Measurements Resin was dried and thoroughly ground in agate pestle and mortar to palatalized isostatically in a steel die at 10 tones/2inch with the help of hydraulic press. A thin layer of colloidal graphite in acetone was applied on both sides of the pellets and dried at room temperature for 4-6 hr. The colloidal graphite on either side of pellets functioned as electrode. The surface continuity of pellet was then tested by means of mutlimeter. The average diameter of this pellets and its thickness were measured using Screw Gauze. Actual dimensions were measured as average of the three measurements taken at three places. -6 -22
Activation Energy (Ea) = 1.48 X 10
Fig.2: Electrical Conductivity Plot of SDBF Resin 4.2 Measurement of Resistivity Hewlett-Packard 4192 Impendance Analyser 5Hz-13MHz was used to measure the electrical conductivity of all resin. The temperature variations of resin were studied by placing the sample holder along with the pallet in the electric furnace and
(ISSN : 2319-6890) 01 April 2013
were then heated slowly. The slow rate of heating 1 to 10 0C per minute was maintained throughout the investigation. Connection wires from the furnace were connected to the terminals of the instrument. The resistances of the sample pallets were measured by two probes (terminals) method. Resistivity (ρ) was then calculated using the relation: ρ = R. x A/l Where, R= resistance of the pellet. A = Surface area of pellets and l = Thickness of pellet. The DC resistivities were measured from 313 to 423 K. The electrical conductivity (σ) varies exponentially with the absolute temperature according to the well-known relationship. σ =σ0 exp –Ea/kT Where, σ =electrical conductivity at room temperature (T) σ0 =electrical conductivity at temperature constant Ea =Activation energy of electrical conduction. K= Boltazmann constant (1.3817x10-23 J mole-1k-1) T= Absolute temperature The relationship has been modified as Log σ = logσ0 + -Ea/2.303kT According to this relation, a plot of Log σ Vs 1/T would be linear with negative slope. From the Slope of the plots, the activation energy was calculated [16-20, 31].
5. RESULTS AND DISCUSSION 5.1 Thermal Degradation Study for SDBF Resin The thermal degradation curve for SDBF resin is shown in Figure1 exhibits four-stage decomposition. First stage was slow and ranged from 40-160oC corresponding to loss 5.6% which may be due to entrapped H2O molecule. The second stage decomposition represents loss of side chain attached to aromatic nucleus and-OH group.[Obs.60.0% againstcalc.59.59%].The third stage decomposition at 240-420 o C which may be due to the loss of -COOH group [observed 78.2% and calculated 77.7%]. The fourth state decomposition is probably total decomposition of resin. The Half Decomposition temperature for SDBF resin is found to be 225oC. By using thermal decomposition data and then applying the Sharp-Wentworth method activation energy has been calculated which is in agreement with the activation energy calculated by Freeman-Carroll method. The thermodynamic parameters have been calculated on the basis of thermal activation energy. These values are incorporated in [Table-1]. Due to abnormally low value of frequency factor [Z] it may be classified as a slow reaction and no other obvious reason can be given. The value of entropy [S] indicates that the activated polymer has more ordered structure than the reactants and the reaction are slower than normal. This is
International Journal of Engineering Research Volume No.2, Issue No.2, pp : 161-166 further supported by low Z values [22- 24, 28, 29].It is very difficult to draw any unique conclusion from the magnitude of thermal activation energy [Ea] as decomposition mechanism is expected to be complicated. Positive values of activation energy under present investigation correspond to the energy of activation due oxidation–reduction process of resin in the higher temperature range [22- 24, 28, 29]. Fairly straight line plots are obtained using the two methods. However, using the Freeman- Carroll method some abnormal points were ignored to get a clear picture about most of the points. Similarly, in the Sharp- Wentworth method, some points at the beginning or the end did not fall on straight line. This is expected, since, the decomposition of resin is not obeying first order kinetics perfectly. These observations are in harmony with the findings of Jacobs and Tompkin and other earlier workers . 5.2 Electrical Conductivity for SDBF Resin The results of electrical conductivity and activation energy are incorporated in Table2. The temperature dependence of the electrical conductivity of the resin has been mentioned in Fig.2.The electrical conduction of polymeric material depends upon incalculable parameters such as porosity, pressure, method of preparation, atmosphere etc; activation energy (Ea) is not affected by these parameters and, therefore, it is fairly reproducible [31-35]. The magnitude of activation energy depends on the number of electrons present in semiconductor materials. The more the number of Л – electrons lowers the magnitude of activation energy and vice versa. Generally polymers containing aromatic nuclei in the backbone exhibit lower activation energy than those with aliphatic system. Thus, the low magnitude of activation energy may be due to the presence of large number of Л-electrons in the polymer chain. This is in good agreement with the most probable structure proposed for the newly synthesized resin under investigation [16-20, 31-35].The carrier motilities of the organic semiconductors might decrease due to: A. The forces between the adjacent molecules are relatively weak as organic compounds from molecular crystals. B. Due to little electronic coupling that exists between the adjacent molecules, it becomes difficult for the electrons to jump from one molecule to other. C. As a consequence of the disordered structure which is due to amorphous nature, the electrons get scattered while traveling through the materials, when they try to flow through it and hence lowers the conductivity. The study shows following results of electrical conductivity1) The electrical conductivity of SDBF resin lies in the range of 1.74 x10-11 to 1.22 x10-7 Siemen.
(ISSN : 2319-6890) 01 April 2013
2) The plots of log versus 1/T is found to be linear in the temperature range under study, which indicate that the Wilson’s exponential law =o exp (E/kT) is obeyed. 3) The energy of activation (Ea) of electrical conduction calculated from the slopes of the plots is found to be in the range of 1.48 x 10-22 J/K. These observations and results are in harmony with the findings of other earlier workers [16-20, 34, 35]
6. CONCLUSION Thermogram of the resin depicts four stages of decomposition. The observed weight loss is little higher than the calculated. This may be due to the degradation of side chain of resin. Activation energy by both Sharp-Wentworth and FreemanCarroll method are in good agreement with each other. Low value of frequency factor [Z] it may be concluded that the reaction of decomposition of resin can be classified as a slow reaction. The negative values for entropy indicate that the activated polymer has more ordered structure than the reactants which are further supported by low Z value. The decomposition of resin is following first order kinetics although not perfectly. Electrical conductivity of this resin increases with increase in temperature which is the important property essential for the resin may be ranked as semiconductors. Hence, this new polymer may be semiconducting in nature.
7. AKNOWLEDGEMENT The authors are thankful to the Head of the Department of Chemistry, Rashtrasant Tukadoji Maharaj Nagpur University, Nagpur for providing necessary laboratory facilities.
Coppo P., Schroeder R., Grell M., Turner M.L.; 771(Organic and Polymeric Materials and Devices), CODEN: MRSPDH; ISSN: 02729172, 2003:61-64. 2. Kang S.W., Kim J.H., Oh K.S., Won J.; J. of Membrane Sc., 2004; 248: 201–206. 3. Nezel T., Fakler A., Zhylyak G., Mohr G.J., Keller S.; Sensors and Actuators B, 2000;70:165–169. 4. Coppo P., Grell M., Turner M.L.; J. Mater. Chem., 2005;15: 1123– 1133. 5. Colin F. P., Rena M. P.; Analytica Chimica Acta ; 1987; 200:151169. 6. Chandra R., Rajabi L., Soni R. K.; J.of Appl. Polym. Sc.; 1996; 62, 4:661-671. 7. MasramD.T.; E- J. of Chemistry; 2009; 6(3):830-834. 8. Das A.P.; S. Lenka; Nayak P.L.; J. Appl. Polym. Sci. 1985; 30:4619. 9. Aristove L.J.; Kostantinov V.V.; Izu. Tomsk. Politekhn. Inst.; 1961; 111: 104-6. 10. Samal R.K.,Senapati B.K. ,Behuray T.B.; J. Appl. Polym. Sci. ; 1996 ; 62 : 655.
International Journal of Engineering Research Volume No.2, Issue No.2, pp : 161-166 11. DeGeiso R.C.; Donaruma L.G.; Tomic, E A., Ind. Eng. Chem. Process Des. Dev., ACS pub.; 1963; 2 (1):43–44. 12. Michael P., Lingala P.; Juneja H., Paliwal L.; J. Appl. polym.Sci.; 2004; 92:2278. 13. Masram D.T., Kariya K.P., Bhave N.S.; E-J. of Chemistry; 2010;7(2), 564- 568. 14. Ozawa T.; Applicability of Friedman Plot; J. Thermal Analysis; 1986; 3l: 547-551. 15. Manvalan R.; Patel M.M.; J. Macromolecular Chem.; 1983; A-20 (9):907-925. 16. Talati A.M and Mistry V.N.;Materials Sc. and Eng. ; 1972; 10 : 287290. 17. Han G., Shi G.; Thin Solid Films; 2007; 515, 17: 6986-699. 18. Kharadi G. J.; Panchani S. C.; Patel K. D.; Int. J.of Polym.Mat.; 2010; 59, 8 : 577 – 587. 19. Kanda S.,Kawaguchi S.; J.Chem.Phy.;1961;34; 1070. 20. Kanda S. , Kawaguchi S.; Bulletin of the Chemical Society of Japan; 1957; 30, 2: 192-193. 21. Masram D.T., Kariya K.P., Bhave N.S.; epolymers; 2007; ISSN 1618-7229, 75. 22. Masram D.T., Kariya K.P., Bhave N.S.; High Perform. Polym; 2010; 22, 8:1004 -1016.
(ISSN : 2319-6890) 01 April 2013
23. Jadhao M.M., Paliwal L.J., Bhave N. S.; J. Appl. Polym. Sci.; 2005, 96, 5; 1605 - 1610. 24. Masram D.T., Kariya K.P., Bhave N.S.; Thermans DAE-BRNS 6th National Symposium & workshop on Thermal Analysis, India; 2008: 329-331. 25. Freeman E.S., Carroll B.J.; Phys. Chem. 1958; 62, 4,: 394–397. 26. Freeman E.S., Anderson D.A.;J. Polym. ; 1961; 54, 159: 253 – 260. 27. Sharp J.B.; Wentworth S.A.;Anal. Chem. 1969; 41 (14): 2060–2062. 28. Coats A.W.; Redfen J.P.; J. of Polym. Sc. Part B: Polymer Letters 2003;3, 11:917 – 920. 29. Ozawa T.; J. Thermal Analysis;1971;12, 3: 150-158. 30. Jacobs P.W.M.; Tompkins F.C.; Chemistry of Solids State, E.G., Garner Publication, London;1955;188. 31. Azaroff L.V.; McGraw Hill Inc. New York ; 1960. 32. Dunlop W.V.;, Wiley, New York; 1957;189. 33. Fanun M.; J.Molecular Liquids; 2007; 135, 1-3:5-13. 34. Masram D.T., Kariya K.P., Bhave N.S;Archives of Applied Science Research; 2010;2(2):153-161. 35. Masram D.T., Kariya K.P., Bhave N.S.; Journal of Chemistry (JC); 2011; 01:1-8.
Table1: Result of thermogravimetric analysis of SDBFresin
Decomposition Temp. (T) 282
Half Decomposition Temp. (T*) 499
Activation Energy kJ/mole SharpFreemanWentwort Carroll h FC SW 26.80 17.2
Kinetic parameters by FC Free Entropy energy frequency change change factor Z ∆S(J) ∆F(kJ) (S-1) 8.3 22.66 994.52
Apparent entropy S*(J) -22.78
Table 2: Evaluation of Activation Energy of Conduction SDBF Resin Diameter of the pellet = 1.287 Surface area of the pellet (A) = r2 = 3.142 x (0.643) 2 = 1.301 cm2 Thickness of pellet (l) = 0.196 cm. A/l = 6.995 cm.
Resistance in Ohm 'R'
Resistivity p = RA/l (Ohm.cm)
Electrical Conductivity σ = 1/ρ (Siemen.cm-1)
313 318 323 328 333 338 343 348
3.1949 3.1447 3.0960 3.0488 3.0030 2.9586 2.9155 2.8736
8.65 X 109 6.33 X 109 4.59 X 109 3.21 X 109 1.46 X 109 9.60 X 108 7.84 X 108 5.67 X 108
5.74 X 1010 4.20 X 1010 3.05 X 1010 2.13 X 1010 9.69 X 109 6.37 X 109 5.20 X 109 3.76 X 109
1.74 X 10-11 2.38 X 10-11 3.28 X 10-11 4.69 X 10-11 1.03 X 10-10 1.57 X 10-10 1.92 X 10-10 2.66 X 10-10
-10.7590 -10.6234 -10.4838 -10.3285 -9.9864 -9.8043 -9.7163 -9.5756
International Journal of Engineering Research Volume No.2, Issue No.2, pp : 161-166 353 358 363 368 373 378 383 388 393 398 403 408 413 418 423
2.8329 2.7933 2.7548 2.7174 2.6810 2.6455 2.6110 2.5773 2.5445 2.5126 2.4814 2.4510 2.4213 2.3923 2.3641
3.96 X 108 2.83 X 108 1.92 X 108 9.47 X 107 8.26 X 107 6.93 X 107 5.31 X 107 3.84 X 107 2.16 X 107 1.39 X 107 9.17 X 106 7.92 X 106 4.40 X 106 2.83 X 106 1.23 X 106
2.63 X 109 1.88 X 109 1.27 X 109 6.29 X 108 5.48 X 108 4.60 X 108 3.52 X 108 2.55 X 108 1.43 X 108 9.23 X 107 6.09 X 107 5.26 X 107 2.92 X 107 1.88 X 107 8.16 X 106
(ISSN : 2319-6890) 01 April 2013 3.80 X 10-10 5.32 X 10-10 7.85 X 10-10 1.59 X 10-9 1.82 X 10-9 2.17 X 10-9 2.84 X 10-9 3.92 X 10-9 6.97 X 10-9 1.08 X 10-8 1.64 X 10-8 1.90 X 10-8 3.42 X 10-8 5.32 X 10-8 1.22 X 10-7
-9.4197 -9.2738 -9.1053 -8.7984 -8.7390 -8.6628 -8.5471 -8.4064 -8.1565 -7.9650 -7.7844 -7.7207 -7.4655 -7.2738 -6.9119